DOI: 10.17188/1294919
title: Materials Data on LiMnV(P2O7)2 by Materials Project

description: LiVMn(P2O7)2 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are four inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.99–2.17 Å. In the second Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.99–2.17 Å. In the third Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.99–2.15 Å. In the fourth Li1+ site, Li1+ is bonded in a see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.96–2.05 Å. There are four inequivalent V5+ sites. In the first V5+ site, V5+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.89–2.05 Å. In the second V5+ site, V5+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.90–2.03 Å. In the third V5+ site, V5+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.89–2.03 Å. In the fourth V5+ site, V5+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.90–2.02 Å. There are four inequivalent Mn2+ sites. In the first Mn2+ site, Mn2+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.94–2.26 Å. In the second Mn2+ site, Mn2+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.93–2.24 Å. In the third Mn2+ site, Mn2+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.93–2.25 Å. In the fourth Mn2+ site, Mn2+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.93–2.29 Å. There are sixteen inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two MnO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 42–46°. There are a spread of P–O bond distances ranging from 1.52–1.61 Å. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two MnO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 30–48°. There are a spread of P–O bond distances ranging from 1.52–1.62 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 33–47°. There are a spread of P–O bond distances ranging from 1.49–1.62 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 38–53°. There are a spread of P–O bond distances ranging from 1.51–1.61 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two MnO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 30–49°. There are a spread of P–O bond distances ranging from 1.52–1.62 Å. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two MnO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 43–49°. There are a spread of P–O bond distances ranging from 1.52–1.62 Å. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 33–48°. There are a spread of P–O bond distances ranging from 1.49–1.63 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 44–53°. There are a spread of P–O bond distances ranging from 1.52–1.61 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two MnO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 43–49°. There are a spread of P–O bond distances ranging from 1.52–1.62 Å. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two MnO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 30–49°. There are a spread of P–O bond distances ranging from 1.52–1.61 Å. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 44–52°. There are a spread of P–O bond distances ranging from 1.52–1.62 Å. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 33–48°. There are a spread of P–O bond distances ranging from 1.49–1.63 Å. In the thirteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two MnO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 46–48°. There are a spread of P–O bond distances ranging from 1.53–1.62 Å. In the fourteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra, corners with two MnO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 31–51°. There are a spread of P–O bond distances ranging from 1.52–1.61 Å. In the fifteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 33–48°. There are a spread of P–O bond distances ranging from 1.50–1.62 Å. In the sixteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, corners with two VO6 octahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 42–52°. There are a spread of P–O bond distances ranging from 1.49–1.63 Å. There are fifty-six inequivalent O2- sites. In the first O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the second O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the third O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one Mn2+ and one P5+ atom. In the fourth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Mn2+ and one P5+ atom. In the fifth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V5+, and one P5+ atom. In the sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the seventh O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one V5+ and one P5+ atom. In the eighth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the ninth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the tenth O2- site, O2- is bonded in a bent 150 degrees geometry to one Mn2+ and one P5+ atom. In the eleventh O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Mn2+ and one P5+ atom. In the twelfth O2- site, O2- is bonded in a bent 150 degrees geometry to one Mn2+ and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the fourteenth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one V5+ and one P5+ atom. In the fifteenth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the sixteenth O2- site, O2- is bonded in a distorted T-shaped geometry to one Li1+, one V5+, and one P5+ atom. In the seventeenth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the eighteenth O2- site, O2- is bonded in a 2-coordinate geometry to one Mn2+ and one P5+ atom. In the nineteenth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Mn2+ and one P5+ atom. In the twentieth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Mn2+, and one P5+ atom. In the twenty-first O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one V5+ and one P5+ atom. In the twenty-second O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V5+, and one P5+ atom. In the twenty-third O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one V5+ and one P5+ atom. In the twenty-fourth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the twenty-fifth O2- site, O2- is bonded in a bent 150 degrees geometry to one Mn2+ and one P5+ atom. In the twenty-sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one Mn2+ and one P5+ atom. In the twenty-seventh O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Mn2+, and one P5+ atom. In the twenty-eighth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the twenty-ninth O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one V5+ and one P5+ atom. In the thirtieth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one V5+ and one P5+ atom. In the thirty-first O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the thirty-second O2- site, O2- is bonded in a distorted T-shaped geometry to one Li1+, one V5+, and one P5+ atom. In the thirty-third O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the thirty-fourth O2- site, O2- is bonded in a 2-coordinate geometry to one Mn2+ and one P5+ atom. In the thirty-fifth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Mn2+ and one P5+ atom. In the thirty-sixth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the thirty-seventh O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one V5+ and one P5+ atom. In the thirty-eighth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V5+, and one P5+ atom. In the thirty-ninth O2- site, O2- is bonded in a distorted bent 120 degrees geome